O R I G I N A L

### Three-dimensional elastic behaviour of common

### yew and Norway spruce

Daniel KeuneckeÆ Stefan Hering Æ Peter Niemz

Received: 6 August 2007 / Published online: 26 April 2008 Springer-Verlag 2008

Abstract In view of its high density, yew wood has a remarkably low longitudinal

Young’s modulus, which makes it unique among coniferous woods. However, the elastic response of yew related to other load directions is largely unknown. Therefore, our goal was to comprehensively characterise the three-dimensional elastic behaviour of yew wood. To achieve this, we performed tensile tests on dog-bone-shaped yew specimens and determined the three Young’s moduli and six Poisson’s ratios using a universal testing machine and a digital image correlation technique. All tests were also applied to spruce as reference species. After including the shear moduli determined in a prior study by our group, all elastic engineering parameters of yew and spruce were ascertained. Based on these values, the three-dimensional elastic behaviour was describable with deformation bodies and polar diagrams. Evaluating these illustrations revealed that yew had a lower stiffness only in the longitudinal direction. In all other three-dimensional directions, spruce was clearly more compliant than yew. Particularly, in the radial–tangential plane, both species varied largely in their degree of anisotropic elasticity. All mentioned dif-ferences between yew and spruce originate at the microstructural level.

Introduction

Yew wood was a very popular longbow wood for hundreds of years, since it fulfils particularly one condition: it is flexible. In the load case of a longbow, ‘flexibility’

means, in technical terms, a low longitudinal Young’s modulus (EL) with

simultaneously large strains in the elastic range. Several literary sources document the relatively low axial stiffness of yew (6,200–12,000 MPa) determined in static

D. Keunecke (*&) S. Hering P. Niemz*

Institute for Building Materials (Wood Physics Group), ETH Zurich, Schafmattstrasse 6, 8093 Zurich, Switzerland

e-mail: danielk@ethz.ch DOI 10.1007/s00226-008-0192-7

tests (e.g., Sekhar and Sharma1959; Jakubczyk1966; Wagenfu¨hr2000; Keunecke

et al. 2007a). In view of its high raw density (620–720 kg m-3 at 11–12%

equilibrium moisture content), this compliant behaviour makes yew wood unique among gymnosperms and an interesting case study for further comprehensive research into its elasticity.

However, clearly less is known about the elastic response of yew related to other load directions. In a first approach, we determined the Young’s and shear moduli of

yew and spruce by means of ultrasonic waves (Keunecke et al.2007b). The radial

(ER) and tangential (ET) Young’s moduli were 2.0–2.3 times higher for yew than for

spruce due to the high density, which was even more intensely reflected in the shear

moduli: GLRand GLTwere three times and GRTsix times higher for yew. Since our

concern is the complete elasto-mechanical characterisation of yew wood, two aspects have to be considered:

• It is well known that the Young’s moduli determined dynamically are

overestimated in contrast to the shear moduli, which are in the same range as the statically determined values.

• The stress–strain relations of wood, regarded as a rhombic crystalline system,

are based on 12 compliance coefficients sij. For their calculation, a full set of

so-called elastic engineering parameters (also referred to as elastic constants) must be available. Thus, in addition to the Young’s and shear moduli, the Poisson’s

ratios mij are also required.

In the present study, therefore, we designed an appropriate ‘‘dog-bone’’ specimen shape and determined the three Young’s moduli and six Poisson’s ratios of yew (Taxus baccata L.) in uniaxial tensile tests at standard climatic conditions (20C, 65% RH). By this means and by taking into account the shear moduli in our prior study, further interpretation of the three-dimensional elastic behaviour was possible, even when the load axis did not coincide with one of the three orthotropic axes L, R and T. For wood, the principle of the latter was shown for the first time by Ho¨rig

(1933) and illustrated in polar diagrams. So as to serve as a reference species and as

a basis for discussion, all of our investigations and evaluations have also been applied to Norway spruce (Picea abies [L.] Karst.). Its mechanical properties are well documented in numerous studies, which proved helpful towards appraising the validity of our results.

In the wood sector, the first sets of elastic engineering parameters have been

determined for spruce (Carrington 1923; Schlu¨ter 1932; Krabbe 1960; Neuhaus

1981). In the meantime, full sets of further softwoods and hardwoods, partly tropical

species, are available. While the determination of Young’s moduli is relatively uncomplicated (e.g., in tensile tests), the shear moduli require much more effort. Direct determination with cubes or discs and indirect determination by means of torsion are reported, as well as the dynamic procedures such as ultrasound and eigenfrequency.

Because of the difficulty in measuring small strains precisely, the Poisson’s ratios of relatively few wood species are available from literature. They have typically been determined using strain gages or inductive strain measurements so far. In this study, a non-contacting optical surface deformation measurement method was

chosen. The major advantages of this digital image correlation (DIC) technique are as follows: (1) the measurement process does not influence the behaviour of the specimen during the test; (2) no restrictions exist regarding the specimen size and geometry; (3) full-field measurements cover inhomogeneous surface deformations as is likely to be present in wood.

With this study, we wanted to

• describe the three-dimensional elastic behaviour of yew wood

• evaluate the main differences between yew and spruce regarding their elasticity

• verify if the chosen experimental setup is appropriate to determine the Young’s

moduli and Poisson’s ratios of wood

Material and methods

Raw material

The centrepieces of the specimens (Fig.1a) were cut from five yew and five spruce

stems (at breast height) grown at stands close to Zurich, Switzerland. The samples were taken from the outer heartwood region where the anatomical structure is approximately orthotropic. Samples containing compression wood were omitted. The 45 centrepieces per species were oriented as follows: 15 9 longitudinal (L), 15 9 radial (R), 15 9 tangential (T).

Specimen composition and shape

Only boards with a thickness of 60–70 mm were available for specimen production; thus, the length in the R and T directions was limited. Since we wanted to produce

Fig. 1 Specimen preparation: a extending the top and bottom ends of the centrepieces by cubes; breinforcing the ends by beech plates; c generating a dog-bone shape using a router; d applying a speckle-pattern; e separating the central part for density measurement. All dimensions in mm

dog-bone-shaped specimens, as they are preferably used in tensile tests, the specimens had to be scaled up to ensure that a feasible minimum number of growth rings were present in the narrow section of the specimens. An influence of inhomogeneity caused by earlywood (EW) and latewood (LW) zones could be reduced this way. Therefore, the centrepieces were extended by gluing cubes of 20 mm edge length to their ends

(Fig.1a). A two-component epoxy adhesive (Araldite) was used for this purpose. The

cubes were of the same wood species as the centrepieces and oriented in the same principle directions. Small beech plates were glued onto the specimens’ ends as lateral reinforcement and to enlarge the load transmission area using again the Araldite

adhesive (Fig.1b). The four-sided dog-bone specimen shape (Fig.1c) was achieved

by a contour template and a router. Consequently, the specimens had vertical and horizontal axes of symmetry. The cross-sectional area in the narrow specimen section was 14 mm 9 14 mm. The section of planar, parallel running specimen surfaces was 11 mm long in the load direction.

Speckle pattern

In the narrow planar specimen section, a filmy high-contrast random dot texture (a ‘‘speckle pattern’’) of 11 mm 9 14 mm was sprayed on two adjacent sides of the

specimen (Fig.1d). To obtain very fine speckles and therefore a high-resolution

pattern, an airbrush gun and finely pigmented acrylic paint was used. First, a white ground coat and then black speckles were applied, resulting in a speckle pattern of heterogeneous grey values. This pattern was needed for the evaluation of displacements on the specimen’s surface during tensile testing by means of the DIC software.

Tensile testing

After the specimens had reached an equilibrium moisture content at 20C and 65% RH, tensile tests were performed using a Zwick Z100 (Schenck) universal testing machine. A load cell with 100 kN maximum capacity was used for L specimens and a 1 kN load cell for R and T specimens. Data acquisition began when a defined pre-load was reached. The tensile tests were performed only at small strains in the linear elastic range. To ensure that plastic deformation was avoided, the specimens were unloaded again at 15% of the predicted maximum load, which had been estimated in preliminary tests. The feed rate was defined such that the maximum load would theoretically be reached in 90 (± 30) s. A total of four loading–unloading cycles was applied to each specimen.

Strain measurement

During tensile testing, one of both speckle fields was filmed by a CCD camera with a distortion-free objective. Vibrations of the camera were avoided. The principle axis of the camera was accurately aligned perpendicular to the specimen surface.

650 9 830 pixels. The image sequences were recorded with a frequency of 4–8 s-1 and saved as TIF files. A cold light source provided even illumination of the speckle field, thereby, too strong reflections from the specimen surface were avoided, which is required for the exact tracking of surface deformation.

After two loading–unloading cycles, the second speckle field was filmed. Exemplified by an L specimen, this means that the camera films the deformations twice on the LR surface and twice on the LT surface.

For subsequent evaluations, the data from the four TIF series per specimen were run through a strain mapping software (VIC 2D, Correlated Solutions) that computed the two-dimensional strain from the surface deformations. The displace-ments are calculated on the basis of a cross-correlation algorithm. Using the grey value pattern in a defined neighbourhood (the ‘‘subset’’) around a central pixel, the algorithm locates the best matching pattern after deformation by maximising the cross-correlation between two subsets. By means of the displacement gradients, strains can be accurately resolved. The resolution of displacement is of the order of 1/100th of a pixel.

After computing the two-dimensional strain, the average strain in the load direction and the average contraction transverse to the load direction was calculated.

Calculation of Young’s moduli

The Young’s modulus E is the ratio of stress (r) to corresponding strain (e) when the

material behaves elastically (Eq.1). It is represented by the slope of the initial

straight segment of the stress–strain diagram:

E¼ Dr=De: ð1Þ

The average stress–strain curve of four loading–unloading cycles in the elastic range was calculated for each specimen.

Calculation of Poisson’s ratios

The phenomenon that lateral contraction of a rod occurs as it elongates is called Poisson’s effect. The ratio of passive (=contraction) to active (=elongation) strain is

defined as Poisson’s ratio mij:

mij¼ ei=ej; ð2Þ

where i refers to the direction of lateral contraction and j to load-directional elongation. Transverse contraction was plotted against load directional strain. The slope of the linear regression multiplied by (-1) corresponds to the Poisson’s ratio. This time, the mean value is based on two measurements.

Calculation of compliance coefficients

Derived from Voigt’s (1928) disquisition on crystal physics, Ho¨rig (1933) idealised

properties related to three orthotropic axes (L, R, T). In such an anisotropic system,

12 compliance coefficients sijare required to describe the three-dimensional elastic

behaviour when the geometric and orthotropic axes coincide. A common notation of Hooke’s law is the compliance matrix equation where strains are stated as linear functions of stresses: e1 e2 e3 c23 c13 c12 0 B B B B B B @ 1 C C C C C C A ¼ s11 s12 s13 0 0 0 s21 s22 s23 0 0 0 s31 s32 s33 0 0 0 0 0 0 s44 0 0 0 0 0 0 s55 0 0 0 0 0 0 s66 2 6 6 6 6 6 6 4 3 7 7 7 7 7 7 5 r1 r2 r3 s23 s13 s12 0 B B B B B B @ 1 C C C C C C A : ð3Þ

By using the concept of strain energy, the 12 compliance coefficients can be even

further simplified to nine independent coefficients (s12= s21, s13= s31, s23= s32).

For details, see for example Bodig and Jayne (1993). The diagonal coefficients sij

(i = j) are reciprocals of the Young’s and shear moduli (the notation is adapted

according to Ho¨rig (1933)):

s11 ¼ E1T ; s22 ¼ E1L ; s33 ¼ E1R ; s44¼ G1LR; s55¼ G1TR; s66¼ G1TL: ð4Þ

The non-diagonal coefficients sij*(i = j) are defined as follows:*

s21¼ s11 mLT; s31¼ s11 mRT; s12¼ s22 mLT; s32¼ s22 mRL;

s13¼ s33 mTR; s23¼ s33 mLR:

ð5Þ

Consequently, all compliance coefficients can also be expressed in terms of engi-neering elastic parameters:

eT
eL
eR
cLR
cTR
cTL
0
B
B
B
B
B
B
B
B
B
@
1
C
C
C
C
C
C
C
C
C
A
¼
1
ET
mLT
EL
mRT
ER 0 0 0
mTL_{ET} 1
EL
mRL
ER 0 0 0
mTR
ET
mLR
EL
1
ER 0 0 0
0 0 0 GLR1 0 0
0 0 0 0 G1TR 0
0 0 0 0 0 GTL1
2
6
6
6
6
6
6
6
6
6
4
3
7
7
7
7
7
7
7
7
7
5
rT
rL
rR
sLR
sTR
sTL
0
B
B
B
B
B
B
B
B
B
@
1
C
C
C
C
C
C
C
C
C
A
: ð6Þ

Density and moisture content

The central cuboid was cut out of each specimen (Fig.1e) and used for

gravimetrical density determination. In this manner, the density of the load-carrying narrow section of the specimens was measured. For the calculation of the

moisture content x (Eq.7), the mass of the cuboids was determined at 20C/65%

RH (mx) and oven-dry (m0):

Results and discussion

Strain measurement

In a preceding evaluation step, the deformation of various sub-areas reduced to one-third of the full speckle field was analysed exemplarily. It was found that – independent from the sub-area position – the strains of sub-areas and the full speckle field were almost identical. Furthermore, there was (if at all) minimal difference between the four individual stress–strain curves measured per specimen.

A representative example for the strain data of a full loading–unloading cycle

provided by the DIC software is shown in Fig.2. In this case, a yew specimen was

loaded longitudinally and the deformations on the LR surface were analysed, i.e., the mean longitudinal strain and mean radial contraction were computed. Even the development of small strains (in this example up to 0.12% and -0.06%) was

reliably trackable due to the sub-pixel accurate algorithm. In Fig.3, longitudinal

strain is plotted against radial contraction for the same data set as shown in Fig.2.

The values decrease in an acceptable narrow path. The slope of the linear regression

(in this case -0.46) multiplied by (-1) corresponds to the Poisson’s ratio mRL.

The aforementioned observations indicate that the specimen shape and the experimental boundary conditions were appropriate for our purposes. Nevertheless, using a second CCD camera and averaging simultaneous strain measurements on the front and back side of the specimen certainly would increase the accuracy of the results.

Young’s moduli

Table1 provides an overview of the determined elastic engineering parameters.

Even though 15 specimens per species and orientation were prepared, the number

Fig. 2 Mean longitudinal strain and mean radial contraction of a loading–unloading cycle computed for a longitudinal specimen

eventually used for data interpretation is partly reduced. In a few cases, the adhesive was not completely hardened, probably due to a slightly deviant mixture ratio between resin and hardener.

The Young’s moduli of spruce are roughly in the range of literature references

(Table2). The mean EL was lower for yew than for spruce (10,500 vs.

12,800 MPa). Calculating the specific EL (=EL related to raw density) would

reveal an even larger difference between both species (17,000 vs. 27,200 MPa/

kg m-3). This is in agreement with our previous studies where we measured ELof

both species in three-point bending (Keunecke et al. 2007a) and dynamically

(Keunecke et al.2007b). Our current investigations with different techniques (X-ray

scattering, pit aperture method) suggest that the microfibril angle (MFA) of the S2

tracheid layer is clearly larger in yew (particularly in LW tracheids) and therefore causes, despite the high density, the low axial stiffness. This relationship between MFA and stiffness is well known and has been shown, for example, by Reiterer

et al. (1999).

In contrast, ER and ETwere about 50% higher for yew compared to spruce. By

means of ultrasonic waves, a 100–130% higher transverse stiffness was determined

for yew than for spruce (Keunecke et al.2007b). Wedge splitting tests performed on

both species (Keunecke et al.2007c) even revealed a 300% higher stiffness for yew.

In that special case, however, this was influenced by the specimen geometry and the presence and position of a starter notch. As becomes clear, transverse stiffness can vary strongly due to the natural heterogeneity of the wood and depending on the measurement method. Nevertheless, in all cases, it was clearly higher for yew than for spruce, predominantly as a result of the high density. Current evaluation of high-resolution X-ray density profiles reveals that particularly the EW zones of yew are

clearly denser (500–600 kg m-3) than those of spruce (250–300 kg m-3) while the

LW density is similar for both species (900–1,000 kg m-3) (Fig.4). However, to a

certain extent, the higher transverse stiffness of yew can also be explained by its

higher MFA. Considering the drastic differences between GRTof yew and spruce, it

seems likely that the species differ in further submicroscopic parameters such as matrix composition or cell/cell adhesion.

The lower axial and higher transverse stiffness of yew is of course reflected in the

quotients EL/ER(=11 for yew and =21 for spruce) and EL/ET(=17 for yew and =32

for spruce), which emphasise the large discrepancy between both species. A further

anatomical feature causes a ratio ER/ETof 1.5 for yew and 1.6 for spruce: wood rays

reinforce the tissue in the radial direction (Burgert2000).

Poisson’s ratios

According to Bodig and Jayne (1993), Poisson’s ratios do not seem to vary with

density or other anatomical characteristics of wood in any recognisable fashion. This may explain why we did not find considerable differences between both

species in this respect (Table1). Only mRLwas higher for yew (0.46) than for spruce

(0.36). In view of the small number of specimens, not too much should be read into

this difference. mRL, mTLand mTRof spruce are comparable with literature references

(Table2). mRT, however, was smaller (0.20 for yew and 0.21 for spruce), resulting in

a ratio mTR/mRT of 2.3 for spruce and 2.5 for yew. According to Eq.8

Table 1 Elastic engineering parameters determined in uniaxial tension Number of specimens n Density q (g cm-3 ) Young’s modulus E (MPa) Poisson’s ratios (–) mRL mTL mTR mRT Yew L x 12 0.62 10,500 0.46 0.48 – – CoV (%) 5.7 13.6 13.2 25.9 R x 15 0.63 927 – – 0.50 – CoV (%) 6.3 24.6 14.8 T x 14 0.62 627 – – – 0.20 CoV (%) 6.1 17.5 30.6 Spruce L x 10 0.47 12,800 0.36 0.45 – – CoV (%) 7.2 9.2 13.2 8.2 R x 13 0.48 625 – – 0.48 – CoV (%) 6.6 20.4 19.2 T x 11 0.46 397 – – – 0.21 CoV (%) 7.2 10.3 16.8

Ta ble 2 Elasti c engi neering and compli ance par ameters: com pariso n o f our mean valu es and li terature referenc es Moi sture cont ent x (% ) Compli ance par ameters Elas tic en gineering par ameters Anis otropy( EL /E T )/ (E L /E R )/( ER /E T ) (–) s11 /s22 /s33 (Pa -1) s44 /s55 /s66 (Pa -1) -s23 /-s13 / -s12 (Pa -1) -s32 /-s31 / -s21 (Pa -1) ET /E L /E R (M Pa) GLR /G RT / GLT (MPa) mLR /mTR / mTL (– ) mRL /mRT / mLT (–) O u r measu rements Ye w 1 1 1,590/9 5/ 1,08 0 575/2,7 20/ 606 44/535 /46 44/324 /46 627/ 10,500/ 927 1,740/3 68/ 1,65 0 0.04 1/ 0.50 / 0.48 0.46/ 0.20 / 0.02 9 17/ 11/1.5 Spru ce 12 2,520/7 8/ 1,60 0 1,621/ 18,9 00/ 1,70 0 28/768 /35 28/528 /35 397/ 12,800/ 625 617/53 /587 0.01 8/ 0.48 / 0.45 0.36/ 0.21 / 0.01 4 32/ 21/1.6 Lite rature refere nces Spru ce (Ho ¨rig 1933 ) 10 2,500/6 2/ 1,43 0 1,590/ 27,0 00/ 1,29 0 27/600 /33 27/600 /33 400/ 16,200/ 699 628/37 /775 0.01 9/ 0.42 / 0.54 0.44/ 0.24 / 0.01 3 41/ 23/1.7 Spru ce (Krabbe 1960 ) 12 2,330/8 8/ 902 1,350/ 27,5 00/ 1,46 0 430/ 11,400/ 1,110 742/36 /686 27/ 10/2.6 Spru ce (Neu haus 1981 ) 12 2,380/8 3/ 1,22 0 1,600/ 23,6 00/ 1,35 0 68/732 /46 37/740 /84 420/ 12,000/ 818 623/42 /743 0.05 6/ 0.60 / 0.55 0.41/ 0.31 / 0.03 5 29/ 15/1.9 Spru ce (Wom melsdo rff 1966 ) 14 2,330/8 9/ 1,02 0 50/598 /50 40/606 /65 429/ 11,300/ 980 0.04 9/ 0.59 / 0.56 0.45/ 0.26 / 0.02 8 26/ 12/2.3 Softw oods (Bodig and Jayne 1993 ) 0.04 1/ 0.47 / 0.42 0.37/ 0.35 / 0.03 3 The shear mo duli in the first (yew) and second ro w (spruce ) have be en determ ined my mean s o f ultra sonic w aves in a prior stu dy (Keunecke et al. 2007b )

mTR m1RT¼ ER E1T ; ð8Þ

mTR/mRT should theoretically be approximately 1.5 taking the determined Young’s

moduli into account. This deviation due to the small mRTprobably results from the

specimen geometry. Especially for tangential specimens, it is difficult to ensure that the growth rings are arranged absolutely parallel to the load direction over the whole specimen length. A solution to this problem could be to produce specimens from several laminated layers to optimise the orthotropic orientation [as done by Krabbe

(1960) or Neuhaus (1981)]. In this study, it was our intention to forgo lamellation to

avoid an influence by the adhesive on the elastic behaviour.

Since the contraction was too small for a satisfactory resolution with the DIC

software, mLRand mLTwere not gaugeable. This is a well known problem in the field

of materials testing (Bodig and Jayne1993). Therefore, it is a common practise to

calculate mLRand mLTaccording to the following relationship:

mLR¼ mRL ER E1L and mLT¼ mTL ET E1L : ð9Þ

mLR= 0.041 and mLT= 0.029 for yew, as well as mLR= 0.018 and mLT= 0.014 for

spruce are obtained from Eq.9.

Compliance parameters sij

Table2provides an overview of the determined elastic engineering and compliance

parameters. The shear moduli are added from our previous study (Keunecke et al.

2007b), where specimens from the same stems as used in this study were tested. Furthermore, literature references for spruce and softwoods in general are listed in

the table. One should note that –s21and –s23were calculated according to Eq. 5, i.e.,

by means of the calculated Poisson’s ratios mLT and mLR. Consequently, the

numerical values of –s12and –s21are identical, as are the numerical values for –s23

and –s32. The asymmetry between –s13and –s31results again from the ratio mTR/mRT.

The mean value (–s13= –s31= 430 Pa-1for yew and 648 Pa-1for spruce) would

probably be closer to the actual value. Alternatively, mRT may be adjusted to

two-thirds the value of mTR.

Three-dimensional elastic behaviour

The compliance matrix (Eq.3) is only valid when stresses and strains are related to

the principle growth directions L, R and T. If they deviate from these axes, the equations describing stress and strain have to be transformed to obtain a statement of Hooke’s law in a three-dimensional coordinate system. A detailed description of the transformation procedure and a first-time spatial illustration as ‘deformation

bodies’ can be found in Grimsel (1999). Two-dimensional sections through these

bodies (as polar diagrams of the LR, LT and RT planes) were already derived at an

early stage by Ho¨rig (1933) on the basis of Voigt’s (1928) textbook on crystal

physics.

In Fig.5, such deformation bodies are presented for yew and spruce based on

coordinate transformations using our values sij in Table2. They have to be

interpreted as follows: To any arbitrary chosen axis in the three-dimensional coordinate system representing the L, R and T directions of a wood species, an identical tensile load is applied. The bodies illustrate the degree of deformation depending on the load direction.

A conspicuous anisotropy of spruce is obvious, as also shown by Grimsel (1999).

The anisotropy of yew is clearly less pronounced; the deformation body rather resembles those shown by Grimsel for beech or mahogany. This is remarkable since, according to Grimsel, all deformation bodies evaluated so far for softwoods show similar characteristics and can clearly be distinguished from those of deciduous trees.

According to Bodig and Jayne (1993), however, comparison of experiment and

theory has shown that a three-dimensional transformation is not always reliable for

Fig. 5 Deformation bodies for yew and spruce. The scale of the axes is adjusted to the respective maximum deformation and thus not identical for both diagrams. Using the same scale would increase the spruce body to the 2.5-fold size (see also Fig.6)

wood, while transformations in the principle planes are usually quite satisfactory. Nevertheless, in our opinion, deformation bodies are a valuable visual aid. Using appropriate software allows their rotation; examination of different perspectives assists in visualising and estimating the approximate spatial elastic characteristics of a wood species.

Two-dimensional polar diagrams (Fig.6) show that yew and spruce only slightly

diverge in the LR and LT plane. The general run of the curves is quite similar even though at a different scale. In contrast, the curves completely differ in the RT plane. Here, the deformation of spruce is highly anisotropic: Even small deviations from the principle axes cause a considerable increase of compliance at the same stress level. The maximum value (a multiple of the deformation along the R and T axes) is

reached at an angle of about 45 as a result of the small GRT. Yew behaves

completely different: the deformation is largest on the T and R axes and slightly decreases to a minimum near 45. Several factors may contribute to the lower directional dependence:

• The density variations between EW and LW are small compared to spruce

(Fig.4).

• The ratios GRT/ERand GRT/ETare clearly higher for yew than for spruce.

Moreover, the tracheids of yew are up to one-third smaller in length and diameter and also show a slightly more rounded cell shape (even in zones free of compression wood) compared to spruce. These aspects possibly support the more homogeneous deformation in the RT plane as well.

Both types of diagrams reveal that the only load direction, where yew is more compliant than spruce, is the L direction and a narrow range around it. However, this just accounts for a fraction of the whole three-dimensional body. In the

Fig. 6 Load-directional dependence of compliance in the principle planes illustrated in three polar diagrams. Each diagram represents a quarter circle

remaining directions yew is clearly stiffer than spruce. This again indicates the enormous impact of the MFA on longitudinal stiffness.

Conclusion

Our results confirm the lower axial and higher transverse stiffness of yew compared to spruce. This present and a prior study by our group complement each other and provide insight into the three-dimensional elasticity of both species. Illustrations such as the three-dimensional deformation bodies assisted in obtaining a general idea of their characteristic spatial compliance. Polar diagrams of the three principle orthotropic planes revealed that the main differences between both species regarding anisotropy are located in the RT plane. Based on both illustration options, yew wood turned out to behave clearly less anisotropic compared to spruce (and probably also compared to most other gymnosperms). Only in the longitudinal direction did yew have a lower stiffness. In all other three-dimensional directions, spruce was clearly more compliant than yew.

The chosen experimental setup was basically well suited to determine the Young’s moduli and Poisson’s ratios of yew and spruce at small strains, even though it leaves room for further development. The specimen shape was appropriate; solely in the case of tangential specimens should improvement measures such as lamellation be considered. With regard to statistical significance, however, a larger number of specimens would be desirable, but this was limited as a consequence of the time-consuming preparation. The accuracy of strain measure-ment based on the combination speckle pattern/CCD camera/DIC software turned out satisfactory for our purposes with a reasonably short computing time.

The main focus of our future investigations will be directed at the question: Is the low axial stiffness of yew also present at lower hierarchical levels (such as microtome sections or individual tracheids)?

Acknowledgments This work was supported by the European Cooperation in the field of Scientific and Technical Research (COST, Action E35).

References

Bodig J, Jayne BA (1993) Mechanics of wood and wood composites. Krieger Publishing Company, Malabar, p 712

Burgert I (2000) Die mechanische Bedeutung der Holzstrahlen im lebenden Baum. Dissertation, Hamburg, p 173

Carrington H (1923) The elastic constants of spruce. Philos Mag 45:1055–1057

Grimsel M (1999) Mechanisches Verhalten von Holz: Struktur- und Parameteridentifikation eines anisotropen Werkstoffes. Dissertation, Dresden, p 89

Ho¨rig H (1933) Zur Elastizita¨t des Fichtenholzes. 1. Folgerungen aus Messungen von H. Carrington an Spruce. Z Tech Phys 12:369–379

Jakubczyk B (1966) Technical properties of the yew wood from the preserve Wierzchlas. Sylwan 10:79–86 Keunecke D, Ma¨rki C, Niemz P (2007a) Structural and mechanical properties of yew wood. Wood Res

Keunecke D, Sonderegger W, Pereteanu K, Luthi T, Niemz P (2007b) Determination of Young’s and shear moduli of common yew and Norway spruce by means of ultrasonic waves. Wood Sci Technol 41:309–327

Keunecke D, Stanzl-Tschegg S, Niemz P (2007c) Fracture characterization of yew (Taxus baccata L.) and spruce (Picea abies [L.] Karst.) in the radial–tangential and tangential–radial crack propagation system by a micro wedge splitting test. Holzforschung 61:582–588

Krabbe E (1960) Messungen von Gleit- und Dehnungszahlen an Holzsta¨bchen mit rechteckigen Querschnitten. Dissertation, Hannover, p 106

Neuhaus FH (1981) Elastizita¨tszahlen von Fichtenholz in Abha¨ngigkeit von der Holzfeuchtigkeit. Dissertation, Bochum, p 162

Reiterer A, Lichtenegger H, Tschegg S, Fratzl P (1999) Experimental evidence for a mechanical function of the cellulose microfibril angle in wood cell walls. Philos Mag A Phys Condens Matter Struct Defects Mech Properties 79(9):2173–2184

Schlu¨ter R (1932) Elastische Messungen an Fichtenholz. Dissertation, Braunschweig, p 56

Sekhar AC, Sharma RS (1959) A note on mechanical properties of Taxus baccata. Indian Forest 85:324–326 Voigt W (1928) Lehrbuch der Kristallphysik. B.G. Teubner, Leipzig, p 960

Wagenfu¨hr R (2000) Holzatlas. Fachbuchverlag Leipzig, Mu¨nchen, p 707